Loading in 5 sec....

Superconductor StabilityPowerPoint Presentation

Superconductor Stability

- 112 Views
- Uploaded on
- Presentation posted in: General

Superconductor Stability

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Superconductor Stability

CERN Accelerator School

Superconductivity for Accelerators

Erice, April 25th – May 4th, 2013

Luca.Bottura@cern.ch

- Training and degradation
- Perturbation spectrum overview
- Heat balance
- Stabilization strategies and criteria
- A summary and more complex topics

focus on LTS magnets

adiabatic, or helium cooled

- Training and degradation
- Perturbation spectrum overview
- Heat balance
- Stabilization strategies and criteria
- A summary and more complex topics

- Superconducting solenoids built from NbZr and Nb3Sn in the early 60’s quenched much below the rated current …
- … the quench current increased gradually quench after quench: training
M.A.R. LeBlanc, Phys. Rev., 124, 1423, 1961.

NbZr solenoid

Chester, 1967

P.F. Chester, Rep. Prog. Phys., XXX, II, 561, 1967.

NbZr solenoid vs. wire

- … but did not quite reach the expected maximum current for the superconducting wire !
- This was initially explained as a local damage of the wire: degradation, a very misleading name.
- All this had to do with stability

Ic of NbZr wire

Imax reached in NbZr solenoid

The prediction of the degraded current […] proved to be impossible and[…] the development of coils passed through a very speculative and empirical phase

P.F. Chester, Rep. Prog. Phys., XXX, II, 561, 1967.

- Training of an model Nb3Sn 11 T dipole for the LHC upgrade in liquid and superfluid helium
- Still, training may be necessary to reach nominal operating current
- Short sample limit is not reached, even after a long training sequence
stability is (still) important !

11 T field in the dipole bore

Courtesy of G. Chlachidze, Fermilab, April 2013, unpublished

- “Those tiny, primitive magnets were, of course, terribly unstable […] One had to have faith to believe that these erratic toys of the low temperature physicist would ever be of any consequence as large engineered devices”(J. Hulm, ASC 1982)

W.B. Sampson, Proc. Int. Symp. Mag. Tech., SLAC, 530-535, 1965

- A six weeks summer study organized and hosted by BNL in 1968
- The crème de la crème addressed material and engineering issues of superconducting accelerators, among them:
- Stability, training and degradation
- Flux-jumps in composite superconductors
- Twisting of multi-filamentary wires and cables

J. Hale

Y. Iwasa

M. Morpurgo

B. Montgomery

W. Sampson

P. Smith

P. Lazeyras

R. Wittgenstein

Approach Jc(T, B, …)

Transition to normal state and Joule heat generation in current sharing

heat generation >

heat removal

no

yes

Stable operating condition

Quench

External perturbation:

flux jump

conductor motions

insulation cracks

AC loss

heat leaks

nuclear

…

Stable operating condition

Heat balance

Perturbation spectrum

stability analysis

and design

- Training and degradation
- Perturbation spectrum overview
- Heat balance
- Stabilization strategies and criteria
- A summary and more complex topics

- Mechanical events
- Wire motion under Lorentz force, micro-slips
- Winding deformations
- Failures (at insulation bonding, material yeld)

- Flux-jumps (important for large filaments, old story ?)
- AC loss (most magnet types)
- Current sharing in cables through distribution/redistribution

- Current leads, instrumentation wires
- Heat leaks through thermal insulation, degraded cooling

- Particle showers in particle accelerator magnets
- Neutron flux in fusion experiments

- Transient (stability concern)
- pointQ [Joules]
- distributedQ’’’[Joules/m3][mJ/cm3]

- Continuous (sizing of cooling system)
- pointq[Watts]
- distributedq’’’[Watts/m3]

After the work of M.N. Wilson, Superconducting Magnets, Plenum Press, 1983

External field change induces screening persistent currents (JC) in the superconductor

A small perturbation induces a temperature increase

B

Critical current density decreases at increasing temperature

JC

A drop in screening current causes the field profile to enter in the superconductor

Energy is dissipated (flux motion)

B

Thermal diffusivity and heat capacity is small in the superconductor and the temperature increases

JC

- During a complete flux-jump the field profile in a superconducting filament becomes flat:
- e.g.: field profile in a fully penetrated superconducting slab
- energy stored in the magnetic field profile:
D = 50 mm, Jc = 10000 A/mm2

area lost during flux jump

Q’’’ 6 mJ/cm3

NOTE: to decrease Q’’’, one can decrease D

Partial flux jump

Complete flux jump

A.D. McInturrf, Composite Materials, Proceedings of the 1968Summer School on Superconducting Devices and Accelerators, BNL 50155 (C-55)

B. Bordini, et al., Magnetization Measurements of High-JC Nb3Sn Strands, CERN-ATS-2013-029

Flux jumps is not an old story, we still suffer from magnetic instabilities when pushing for high conductor JC

- Training and degradation
- Perturbation spectrum overview
- Heat balance
- Stabilization strategies and criteria
- A summary and more complex topics

Heat source

Joule heat

Conduction

cooling

generation

Heat capacity

Heat transfer

…effect of heat conduction and cooling…

…decision time…

heat pulse Q’’’ext…

Q’’’ext = Q’’’+e

generation > cooling

Q’’’ext = Q’’’-e

generation < cooling

- Q’’’, energy margin
- Minimum energy density that leads to a quench
- Maximum energy density that can be tolerated by a superconductor, still resulting in recovery
- Simple and experimentally measurable quantity (…)
- Measured in [mJ/cm3] for convenience (values 1…1000)
- Also called stability margin
- Compared to the energy spectrum to achieve stable design

- Q, quench energy
- Better adapted for disturbances of limited space extension
- Measured in [mJ] to [mJ]

typical NbTi

Jc

3000 A/mm2

4.2 K

5 T

9 K

14.5 T

T

B

J

operating plane

Jc

Margin in critical current

Bmax

Jop

Margin along the loadline

B

Bop

Bc

J

Margin in temperature

Tcs

Jop

Jop/JC ≈ 0.5

Bop/Bmax ≈ 0.8 (Todesco’s 80 %)

Tcs-Top≈ 1…2 K

Top

Tc

T

fast !!!

15 mV

2 ms

…cooling…

…decision time…

Voltage increase generated by a sudden heat input

…quench

What happens here ?

T < Tcs

Tcs < T < Tc

Ic

T > Tc

Iop

Top

Tcs

Tc

T

stabilizer

superconductor

curent sharing

quenched

Iop

Top

Tc

T

Tcs

current in superconductor

current in stabilizer

- Linear approximation for Ic(T):
- Joule heating

Top

Tc

T

Tcs

- Indirect: (adiabatic, no cooling)
- Contact to a heat sink through conduction (e.g. to a cryo-cooler)
- In practice, no cooling on the time scale of interest for stability

- Direct: (cooling by heat transfer at the surface)
- Bath cooling, to a pool of liquid helium at atmospheric pressure and saturation temperature (4.2 K)
- Force-flow cooling to a supercritical or two-phase flow
- Superfluid cooling to a stagnant bath of He-II

- Training and degradation
- Perturbation spectrum overview
- Heat balance
- Stabilization strategies and criteria
- A summary and more complex topics

Top

Tc

T

Tcs

- Adiabatic conditions:
- No cooling (dry or impregnated windings)
- Energy perturbation over large volume (no conduction)

energy margin

volumetric enthalpy

30

3

2

2

enthalpy reserve increases at increasing T (Note: HTS !)

do not sub-cool !

(if you can only avoid it…)

- Applies to:
- Adiabatic, compact, high current density windings (dry or indirectly cooled)
- Very fast heat perturbations (flux-jumps)

- The heat capacity of the conductor absorbs the external heat perturbation
- Stability (at equal temperature margin) improves as the temperature increases (HTS !)
- Choose materials with high heat capacity (e.g. loading of epoxy)
- Relatively small energy margin: 1…10 mJ/cm3

A.R. Krantowitz, Z.J.J. Stekly, Appl. Phys. Lett., 6, 3, 56-57, 1965.

Z.J.J. Stekly, J.L. Zar, IEEE Trans. Nucl. Sci., 12, 367-372, 1965.

- Cooling in a bath of pool boiling helium
- Ignore conduction for large energy perturbations volumes
- Request steady state stability in all conditions

worst possible case

cooling

generation

constant heat transfer to the helium

not cryostable

not cryostable

cryostable

cooling

stable

generation

- Steklycryostability condition:
- can be formulated as aStekly 1 :

Decrease the operating current

Improve cooling

Increase the temperature margin

Increase the cross section of stabilizer

- Applies to:
- Well-cooled, low current density windings (pool-boiling)
- Any type of heat perturbations, all time and space scales

- The coolant can take the Joule heating under all possible conditions
- Ideally infinite energy margin

- Assume that the normal zone is long and above cryostable operating conditions
- The temperature will reach an equilibrium temperature

Teq

not cryostable

cryostable

T

T

Teq

Teq

Tc

Tc

Tcs

Tcs

Top

Top

x

x

- What happens if the ends are cold ?
- Request steady state stability in all conditions

cold-end conduction lead to recovery

cold-end conduction not sufficient to prevent quench

t

t

T

Teq

Tc

Tcs

Top

x

Sop = 0 Seq = 0

B.J. Maddock, G.B. James, W.T. Norris, Cryogenics, 9, 261-273, 1969.

- introduce a new variable S:

A/w q’’’J

q’’

wh(T-Top)

x

B.J. Maddock, G.B. James, W.T. Norris, Cryogenics, 9, 261-273, 1969.

Stable conditions are obtained when the net area between generation and cooling curves is zero

Values of a nearly twice as large as from the Stekly criterion are possible !

Stekly: a ≤ 1

Maddock:a≤ 2-fop

- Applies to:
- Well-cooled, low current density windings (pool-boiling)
- Any type of heat perturbations, all time and space scales

- The coolant and the cold ends take the Joule heating under all possible conditions
- Ideally infinite energy margin
- Improved stability with respect to the cryostability condition, allow operation at higher current

- Adiabatically stabilized conductors:
- High Jop (good for cost)
- Small Q’’’ (bad for large magnets)

- Cryo-stabilized conductors (including cold-ends):
- Large Q’’’, ideally infinite (good for large magnets)
- Low Jop (bad for cost)
Is there a compromise ?

The helium heat capacity is orders of magnitude larger than for metals at low temperature

Add helium in intimate contact with the cable

M.O. Hoenig, Y. Iwasa, D.B. Montgomery,

Proc. 5th Magn. Tech. Conf., Frascati, 519, (1975)

- Conductor temperature:
- But the helium temperature evolves as well:
- Under which conditions the heat capacity is effectively used ?
NOTE: at large enough h, TThe

J.W. Lue, J.R. Miller, L. Dresner, J. Appl. Phys., 51, 1, 772, (1980)

J.H. Schultz, J.V. Minervini, Proc. 9th Magn. Tech. Conf., Zurich , 643, (1985)

Joule heat

<

cooling

Joule heat

>

cooling

balance of Joule heat and cooling at:

DQ’’’

well-cooled

helium + strand

heat capacity

equivalent to aStekly = 1

In this case however the CICC is meta-stable as a large enough energy input will cause a quench !

ill-cooled

strand

heat capacity

llim

Iop

T

T’eq

Tc

Tcs

Top

x

q’’

x

Short normal zone

S=0 at the boundaries

equal area still possible

but implies lower T’eq< Teq

A/wq’’’J

wh (T-Top)

T

q’’’J

x

- The temperature profile can be traced by numerical integration of the equal areabalance
- This is an unstable equilibrium temperature profile, and defines the minimum length of superconductor that could grow and develop into a quench: Minimum Propagating Zone (MPZ)
- The energy required to form the MPZ is the Minimum Quench Energy (MQE)

M.N. Wilson, Y. Iwasa, Cryogenics, 18, 17-25, 1978

After the work of M.N. Wilson, Superconducting MagnetsPlenum Press, 1983

- To estimate the size of the MPZ we can solve the heat balance approximately
- Steady state conditions and no cooling

Jop = 400 A/mm2

k = 500 W/m K

h = 1 nW m

TC-Top = 2 K

MPZ ≈ 3.5 mm

MQE ≈ 10 mJ

- Training and degradation
- Perturbation spectrum overview
- Heat balance
- Stabilization strategies and criteria
- A summary and more complex topics

- Superconductor stability is the art of balancing large stored energies (and potential for energy release) with a little capital (aka: “leveraging” for our US colleagues)
- Extremely important in LTS-based magnet to reach the desired performance (10 MJ vs 10 mJ)
- Generally not an issue for HTS-based magnets

- Stability is not absolute, it implies comparing the perturbation spectrum to the available margin
- Several strategies can be applied to achieve stable operating conditions under the envelope of foreseeable perturbation spectrum

Cold end

1000

CICC

Cryostable

100

Energy margin (mJ/cm3)

Adiabatic

10

MPZ/MQE

1

1

10

100

1000

Operating current density (A/mm2)

There are more things in heaven and earth, Horatio, Than are dreamt of in your philosophy.

- Current distribution and RRL
- Ramp-rate quenches
- Holding quenches

- Magneto-thermal instabilities
- Dynamic stability
- Self-field instability

type B

type A

A. Devred, T. Ogitsu, Frontiers of Accelerator Magnet Technology, World Scientific, 184, 1996

B. Bordini and L. Rossi, IEEE TAS, 19, 2470 (2009).

power transmission cables

Strands and tapes

CICC’s

Rutherford

induced flow,

transient heat transfer,

AC operation,

current distribution,

HTS,

coolants (N2, Ne, H2)…

Internally cooled

Things can get fairly complex

Then, you need to protect !

- Papers, reviews and proceedings:
- A.R. Krantowitz, Z.J.J. Stekly, A New Principle for the Construction of Stabilized Superconducting Coils, Applied Physics Letters, 6, 3, 56-57, 1965.
- P.F. Chester, Superconducting Magnets, Rep. Prog. Phys., XXX, Part II, 561-614, 1967.
- B.J. Maddock, G.B. James, W.T. Norris, Superconductive Composites: Heat Transfer and Steady State Stabilization, Cryogenics, 9, 261-273, 1969.
- M.N. Wilson, Y. Iwasa, Stability of Superconductors against Localized Disturbances of Limited Magnitude, Cryogenics, 18, 17-25, 1978.
- L. Dresner, Superconductor Stability 1983: a Review, Cryogenics, 24, 283, 1984.

- M.N. Wilson, Superconducting Magnets, Plenum Press, 1983.
- L. Dresner, Stability of Superconductors, Plenum Press, 1995.
- P.J. Lee ed., Engineering Superconductivity, J. Wiley & Sons, 2001.
- B. Seeber ed., Handbook of Applied Superconductivity, IoP, 1998.
- Y. Iwasa, Case Studies in Superconducting Magnets, Plenum Press, 1994.